Upconversion luminescence of an insulator involving a band to band multiphoton excitation process

A multiphoton process to the conduction band of the insulator Er2O3 is reported, which occurs in vacuum under near infrared excitation. The enormous upconversion intensity is two orders of magnitude greater than that in air, and also the intensity ratio for green and red emission bands is inverted. The mechanism is probed by experiments of laser power dependence, cathodoluminescence, photoconductivity dependence and chemical dilution, and it involves cross-relaxation energy transfer upconversion of erbium ions to reach the conduction band. The upconversion color is tunable by changes in pressure, laser diode intensity and wavelength, or dopant ion concentration. ©2011 Optical Society of America OCIS codes: (170.6280) Spectroscopy, fluorescence and luminescence; (160.5690) Rare-earthdoped materials; (140.3613) Lasers, upconversion; (040.5150) Photoconductivity; (140.6810) Thermal effects. References and links 1. E. Desurvire, Erbium-Doped Fiber Amplifiers: Principles and Applications (John Wiley & Sons, 1994). 2. F. Auzel, “Upconversion and anti-Stokes processes with f and d ions in solids,” Chem. Rev. 104(1), 139–174 (2004). 3. D. Casanova, C. Bouzigues, T.-L. Nguyên, R. O. Ramodiharilafy, L. Bouzhir-Sima, T. Gacoin, J. P. Boilot, P.-L. Tharaux, and A. Alexandrou, “Single europium-doped nanoparticles measure temporal pattern of reactive oxygen species production inside cells,” Nat. Nanotechnol. 4(9), 581–585 (2009). 4. D. R. Gamelin and H. U. Gudel, “Upconversion processes in transition metal and rare earth metal systems,” Top. Curr. Chem. 214, 1–56 (2001). 5. S. Sivakumar, F. C. van Veggel, and M. Raudsepp, “Bright white-light through up-conversion of a single NIR source from sol–gel-derived thin film made with Ln-doped LaF3 nanoparticles,” J. Am. Chem. Soc. 127(36), 12464–12465 (2005). 6. F. Wang, Y. Han, C. S. Lim, Y. Lu, J. Wang, J. Xu, H. Chen, C. Zhang, M. Hong, and X. Liu, “Simultaneous phase and size control of upconversion nanocrystals through lanthanide doping,” Nature 463(7284), 1061–1065 (2010). 7. E. Beurer, J. Grimm, P. Gerner, and H. U. Güdel, “New type of near infrared to visible photon upconversion of Tm -doped CsCaI3,” J. Am. Chem. Soc. 128(10), 3110–3111 (2006). 8. C. Cao, W. Qin, J. Zhang, Y. Wang, P. Zhu, G. Wei, G. Wang, R. Kim, and L. Wang, “Ultraviolet upconversion emissions of Gd,” Opt. Lett. 33(8), 857–859 (2008). 9. S. Schietinger, L. S. Menezes, B. Lauritzen, and O. Benson, “Observation of size dependence in multicolor upconversion in single Yb, Er codoped NaYF4 nanocrystals,” Nano Lett. 9(6), 2477–2481 (2009). 10. W. Kaiser and C. B. Garrett, “Two-photon excitation CaF2: Eu ,” Phys. Rev. Lett. 7(6), 229–231 (1961). 11. D. Jia, L. Liu, and W. M. Yen, “Erbium energy levels relative to the band gap of gadolinium oxide,” Opt. Commun. 212(1-3), 97–100 (2002). 12. W. S. Mallory, “The distribution of energy in the spectrum of erbium oxide,” Phys. Rev. 14(1), 54–66 (1919). 13. Z. L. Wang, H. L. W. Chan, H.-L. Li, and J. H. Hao, “Highly efficient low-voltage cathodoluminescence of LaF3:Ln (Ln=Eu ,Ce,Tb) spherical particles,” Appl. Phys. Lett. 93(14), 141106 (2008). 14. H. L. Li, Z. L. Wang, S. J. Xu, and J. H. Hao, “Improved performance of spherical BaWO4: Tb 3+ phosphors for field-emission displays,” J. Electrochem. Soc. 156(5), J112–J116 (2009). #144563 $15.00 USD Received 21 Mar 2011; revised 9 May 2011; accepted 26 May 2011; published 1 Jun 2011 (C) 2011 OSA 6 June 2011 / Vol. 19, No. 12 / OPTICS EXPRESS 11753 15. P. A. Tanner and K. L. Wong, “Synthesis and spectroscopy of lanthanide ion-doped Y2O3,” J. Phys. Chem. B 108(1), 136–142 (2004). 16. C. K. Jørgensen, H. Bill, and R. Reisfeld, “Cathodoluminescence of rare earth,” J. Lumin. 24-25, 91–94 (1981). 17. J. Wang and P. A. Tanner, “Upconversion for white light generation by a single compound,” J. Am. Chem. Soc. 132(3), 947–949 (2010). 18. C. Brandt, S. T. Fredrich-Thornton, K. Petermann, and G. Huber, “Photoconductivity in Yb-doped oxides at high excitation densities,” Appl. Phys. B 102(4), 765–768 (2011).


Introduction
The lanthanide ion erbium, Er 3+ , is well known for its optical communication applications [1] and two-photon upconversion processes [2] with a quantum efficiency surpassing values for other Ln 3+ ions [3].The mechanisms are mainly based upon excited state absorption (ESA), energy transfer upconversion (ETU) and photon avalanche (PA) for Er 3+ or Er 3+ , Yb 3+ ion codoped systems [2,4].Efforts to improve the quantum efficiency of upconversion have largely focused upon the selection of a suitable host for this activator ion.Oxide and fluoride host lattices, such as LaF 3 , Y 2 O 3 and NaYF 4 are well studied since their relatively low phonon frequencies inhibit nonradiative pathways [5].Here, we report a novel multiphoton upconversion to the conduction band of Er 2 O 3 which occurs in vacuum under near infrared (NIR) excitation and which results in an enormous increase in intensity and obvious change in emission spectra.The upconversion emission color can be tuned by pressure, laser diode intensity, excitation wavelength, or chemical modification.
The lanthanides are long known as the lighting elements and the present article illuminates their burgeoning importance.Concerning their upconversion investigations, the following topics have been of wide interest in recent years: tuning upconversion nanoparticles by lanthanide doping to access a wide emission range from the visible to near infrared regions [6], utilizing the transitions of highly excited 5d [7] or 4f N [8] energy levels; and producing white light upconversion by the combination of several 4f N -4f N transitions of lanthanide ions [5].Most importantly, the improvement in upconversion efficiency has been enthusiastically pursued by different means, such as by using noble metal surface plasmon-enhancement [9].The three basic upconversion mechanisms have not previously been utilized to excite lanthanide ion electrons to the conduction band via a multiphoton process.Part of the reason for this is that the multiphoton upconversion efficiency decreases dramatically when compared with a two photon process [10].As a move in these directions, we present in this work the upconversion luminescence of Er 2 O 3 involving a band to band multiphoton excitation process.In vacuum, the green and red upconversion and near infrared (NIR) emission were observed to be more than two orders of magnitude stronger than in air.The upconversion mechanism involves excitation from within the valence band (VB) to the conduction band (CB) with the simultaneous production of photoconductivity, as also shown by the dependence of upconversion emission intensity upon incident laser power.This mechanism is expected to be applicable to other lanthanide sesquioxides with interband metastable states of the 4f N configuration.edge of slab through the window of the chamber.A Keithley 6517A electrometer was used as the voltage supply and resistance detector.

Comparison of luminescence under cathode-ray and near infrared excitation
Electron-beam excitation may produce orders-of-magnitude greater carrier generation rates than optical excitation, and it is advantageous in studies of wide band-gap materials.The band gap of Er 2 O 3 is located at 5.0 ± 0.6 eV (35490-45170 cm 1 ) [11].The cathodoluminescence (CL) spectra of Er 2 O 3 in vacuum under various beam voltage and beam current values are shown in Figs.1(a) and 1(b).As previously published [12], it is thus demonstrated that aboveband gap excitation leads to visible emission from electronic energy levels of Er 3+ .These extensive spectral bands are assigned to emissions from the 4 G 11/2 / 2 G 9/2 (ultraviolet), 4 F 7/2 (blue), 2 H 11/2 , 4 S 3/2 (green), 4 F 9/2 (red) and 4 I 9/2 (NIR) J-multiplets to the 4 I 15/2 electronic ground state, as marked in Fig. 1(a).These levels are therefore populated by various nonradiative processes from the conduction band (CB) and from interband trap levels.The total Er 3+ emission intensity increases with both excitation voltage and current, similar to the studies of other systems [13,14].but the red/green emission intensity ratio decreases with increase of each of these parameters.Emission from higher multiplet terms of Er 3+ is quenched by crossrelaxation processes in this concentrated material.Figure 1(c) compares the 4f 11 upconversion luminescence from the same high purity Er 2 O 3 powder in air (left hand ordinate scale) and vacuum (right hand ordinate) environments when employing a 975 nm (10256 cm 1 ; 1.27 eV) laser diode with excitation power of 750 mW.Red emission, λ max 660 nm: 4 F 9/2  4 I 15/2 , is dominant in air and the green emission, λ max 564 nm: 2 H 11/2 , 4 S 3/2  4 I 15/2 , is very weak.However in a modest vacuum of up to 2 × 10 2 mbar, the intensity of red emission increases by two orders of magnitude, and the intensity ratio of green to red emission increases considerably so that the intensities of these emissions now become comparable.
The sample temperature may be readily calculated from the comparison of the relative intensities of the emission transitions from 2 H 11/2 and 4 S 3/2 .The comparison of the "air" spectrum [Fig.1(c)] with the literature spectrum [15] shows that the sample temperature under 750 mW laser diode excitation in air is ~500 K, and in "vacuum" it is ~800 K.This elevated temperature partly accounts for the differences in the "air" and "vacuum" spectra in Fig. 1(c), where the former are more clearly resolved and the latter include more transitions from thermally-excited luminescent states.The most important point, however, concerns the similarity between Figs. 1(a) and 1(b) on the one hand, and 1(c) "vacuum", although the former are excited by radiation above, and the latter below, the band gap.Following this observation, we now show that just as for the spectra in Figs.1(a) and 1(b), that in Fig. 1(c) also results from initial excitation into the conduction band.Note that candoluminescence is negligible at 800 K [12,16].

Dependence of laser power, photoconductivity and chemical dilution
The log-log plots of integrated emission intensity for the wavelength range between 400 and 850 nm, versus laser diode power, for the sample in air or vacuum are shown in Fig. 2(a).The slopes of the plots are an indication of the number of photons involved in the upconversion processes, given certain conditions described by Gamelin and Güdel [4].The laser diode radiation is absorbed by a 4f 11  4f 11 intraconfigurational transition, and in the present case it is the 4 I 15/2  4 I 11/2 transition of Er 3+ .The "vacuum" plot in Fig. 2(a) is consistent with ground state absorption to the CB involving 6 (1.27 eV, 10256 cm 1 ) photons.
Excitation to the conduction band is accompanied by the production of free charge carriers.The measurement of electrical conduction by the insulator Er 2 O 3 under NIR irradiation was performed by inserting an electrode at each side of a lightly-compressed disc of the powder.In fact, as shown in Fig. 2(b) for three different ambient pressures, there is a large increase in the current detected when irradiating Er 2 O 3 with increasing laser diode powers, with a variable slope which depends upon the laser power.For 0.05 mbar pressure an avalanche increase to a slope value near 20 occurs for laser diode powers above 750 mW.The photocurrent is very sensitive to ambient pressure, as shown in Fig. 2(c), which may indicate that charge carriers are at the surface, rather than the bulk, of the material.Figure 2(c) also demonstrates that the upconversion emission intensity and photoconductivity are inter-related, although the emission slope has no "bend".The upconversion enhancement under 975 nm excitation does not occur for (Y 0.95 Er 0.05 ) 2 O 3 so that a cross-relaxation process is implied to be responsible for upconversion to the conduction band in the neat Er 2 O 3 powder.Also, we have conducted further experiments in "air" at elevated temperatures to show that the higher sample temperature in "vacuum", mentioned above, is not responsible for the enhancement of upconversion.Figure 1(a) shows that the highest metastable states in Er 2 O 3 are 2 H 11/2 , 4 S 3/2 , which may be reached by a 2-photon process from 4 I 15/2 .A collective energy transfer from three Er 3+ ions excited in these states (i.e. a 6-photon process) could raise an electron from the valence band into the conduction band.The observation of Er 3+ emission demonstrates that nonradiative population of interband states follows the excitation.
It has been demonstrated [17] that quenching of Yb 2 O 3 broad band emission by gas molecules can be interpreted under a model focusing upon the number of collisions by gas molecules irrespective of the nature of the gas.The emission was characterized by a characteristic pressure (P 0 ) which was linearly dependent upon the laser power and the square root of the mass of the ambient gas molecules.The additional results from the present work suggest that the most important action of these gas molecules is surface charge neutralization, thus depleting the occupation of the CB.

Measured luminance and calculated CIE coordinates
Luminance measurements were performed for the same powder sample of Er 2 O 3 under various excitation regimes.For CL under 6.0 kV with 1.5 A beam current, the luminance was 6000 cd m 2 ; whereas under NIR 1 W excitation power, the luminance was 30000 cd m 2 for 975 nm upconversion and 70000 cd m 2 for 808 nm upconversion, as displayed in Fig. 3.
Considering that the luminance of a commercial fluorescent lamp or white LED is around 30000 cd m 2 , the luminance of upconversion is extraordinary.Employing 975 nm laser excitation with 950 mW power, the luminous efficacy is ~4 lm W 1 .The corresponding value is 14 lm W 1 using 808 nm laser excitation and the color coordinate is closer to white emission compared with that of 975 nm upconversion.

Conclusions
In summary, the use of vacuum leads to much more intense upconversion emission in Er 2 O 3 than in air.This behavior is not followed in the diluted Er 3+ system Y 2 O 3 :Er 3+ .The similarity of the emission with that obtained using above band gap excitation, as well as the power dependence of emission intensity and the production of photocurrent, show that upconversion to the conduction band has been achieved.The luminance under NIR excitation is spectacular and the emission color can be tuned by various means.A reviewer has drawn our attention to a recent paper by Brandt et al. [18] which reports photoconductivity under NIR excitation for oxides which are heavily-doped in Yb 3+ .Our analogous results support electron transport in the CB, rather than hole transport in the VB.

Fig. 2 .
Fig. 2. Log-log plots of various experimental variables for Er2O3 powders: (a) integrated emission intensity versus 975 nm laser diode power in the region between 400 and 850 nm in ambient air or vacuum of 2 × 10 2 mbar; (b) photocurrent versus laser power for three pressures; c) photocurrent and upconversion intensity versus pressure using 950 mW NIR laser excitation power: these results are not simultaneous.

Fig. 3 .
Fig. 3. Calculated Commission Internationale de L'éclairage (CIE) coordinate ranges of Er2O3 powder sample under electron gun (CL) and NIR excitation.The circle is for CL; the triangle region for 808 nm excitation and the rectangle for 975 nm excitation.The insets are photographs of Er2O3 powder in a circular metal holder behind a glass window of the vacuum chamber: (top) of the upconversion under 975 nm excitation, (bottom) of the upconversion under 808 nm excitation and (left) of CL.